Bessemer process - wikipedia Bessemer process Bessemer converter, schematic diagram The Bessemer process was the first inexpensive industrial process for the mass production of steel from molten pig iron before the development of the open hearth furnace. The key principle is removal of impurities from the iron by oxidation with air being blown through the molten iron. The oxidation also raises the temperature of the iron mass and keeps it molten. Related decarburizing with air processes had been used outside Europe for hundreds of years, but not on an industrial scale. One such process has existed since the 11th century in East Asia, where the scholar Shen Kuo of that era described its use in the Chinese iron and steel industry. In the 17th century, accounts by European travelers detailed its possible use by the Japanese. The modern process is named after its inventor, the Englishman Henry Bessemer, who took out a patent on the process in 1856. The process was said to be independently discovered in 1851 by the American inventor William Kelly, though there is little to back up this claim. The process using a basic refractory lining is known as the `` basic Bessemer process '' or `` Gilchrist -- Thomas process '' after the English discoverers Percy Gilchrist and Sidney Gilchrist Thomas. Contents 1 Details 1.1 Oxidation 1.2 Managing the process 2 Predecessor processes 3 History 4 Patent battles 5 Importance 6 The Bessemer process in the United States 7 Obsolescence 8 See also 9 References 9.1 Bibliography 10 External links Details Bessemer converter components. Oxidation The blowing of air through the molten pig iron introduces oxygen into the melt which results in oxidation, removing impurities found in the pig iron, such as silicon, manganese, and carbon in the form of oxides. These oxides either escape as gas or form a solid slag. The refractory lining of the converter also plays a role in the conversion -- clay linings are used when there is little phosphorus in the raw material - this is known as the acid Bessemer process. When the phosphorus content is high, dolomite, or sometimes magnesite, linings are used in the alkaline Bessemer limestone process. These are also known as Gilchrist - Thomas converters, after their inventors, Percy Gilchrist and Sidney Gilchrist Thomas. In order to produce steel with desired properties, additives such as spiegeleisen ( a ferromanganese alloy ), can be added to the molten steel once the impurities have been removed. Managing the process When the required steel had been formed, it was poured into ladles and then transferred into moulds while the lighter slag was left behind. The conversion process, called the `` blow '', was completed in approximately 20 minutes. During this period the progress of the oxidation of the impurities was judged by the appearance of the flame issuing from the mouth of the converter. The modern use of photoelectric methods of recording the characteristics of the flame greatly aided the blower in controlling final product quality. After the blow, the liquid metal was recarburized to the desired point and other alloying materials were added, depending on the desired product. A Bessemer converter could treat a `` heat '' ( batch of hot metal ) of 5 to 30 tons at a time. They were usually operated in pairs, one being blown while another was being filled or tapped. Predecessor processes Bessemer converter at Högbo Bruk, Sandviken. Before the Bessemer process, Western Europe and the United States relied on the puddling process to reduce the carbon content of white cast iron ( refined pig iron ), converting it to wrought iron. It was possible to make low - quality puddled steel, but the process was difficult to control and quality varied. High - quality steel was made by the reverse process of adding carbon to carbon - free wrought iron, usually imported from Sweden. The manufacturing process, called the cementation process, consisted of heating bars of wrought iron together with charcoal for periods of up to a week in a long stone box. This produced blister steel. The blister steel was put in a crucible with wrought iron and melted, producing crucible steel. Up to 3 tons of expensive coke was burnt for each ton of steel produced. Such steel when rolled into bars was sold at £ 50 to £ 60 ( approximately £ 3,390 to £ 4,070 in 2008 ) a long ton. The most difficult and work - intensive part of the process, however, was the production of wrought iron done in finery forges in Sweden. This process was refined in the 18th century with the introduction of Benjamin Huntsman 's crucible steel - making techniques, which added an additional three hours firing time and required additional large quantities of coke. In making crucible steel, the blister steel bars were broken into pieces and melted in small crucibles, each containing 20 kg or so. This produced higher quality crucible steel but increased the cost. The Bessemer process reduced the time needed to make steel of this quality to about half an hour while requiring only the coke needed initially to melt the pig iron. The earliest Bessemer converters produced steel for £ 7 a long ton, although it initially sold for around £ 40 a ton. History Bessemer converter, Kelham Island Museum, Sheffield, England ( 2010 ). A system akin to the Bessemer process has existed since the 11th century in East Asia. Economic historian Robert Hartwell writes that the Chinese of the Song Dynasty innovated a `` partial decarbonization '' method of repeated forging of cast iron under a cold blast. Sinologist Joseph Needham and historian of metallurgy Theodore A. Wertime have described the method as a predecessor to the Bessemer process of making steel. This process was first described by the prolific scholar and polymath government official Shen Kuo ( 1031 -- 1095 ) in 1075, when he visited Cizhou. Hartwell states that perhaps the earliest center where this was practiced was the great iron - production district along the Henan - Hebei border during the 11th century. In the 15th century the finery process, another process which shares the air - blowing principle with the Bessemer process, was developed in Europe. In 1740 Benjamin Huntsman developed the crucible technique for steel manufacture, at his workshop in the district of Handsworth in Sheffield. This process had an enormous impact on the quantity and quality of steel production, but it was unrelated to the Bessemer - type process employing decarburization. Johan Albrecht de Mandelslo described the Japanese use of the Bessemer process. The Japanese may have made use of the Bessemer process, which was observed by European travelers in the 17th century. The adventurer Johan Albrecht de Mandelslo describes the process in a book published in English in 1669. He writes, `` They have, among others, particular invention for the melting of iron, without the using of fire, casting it into a tun done about on the inside without about half a foot of earth, where they keep it with continual blowing, take it out by ladles full, to give it what form they please. '' According to historian Donald Wagner, Madelslo did not personally visit Japan, so his description of the process is likely derived from accounts of other Europeans who had traveled to Japan. Wagner believes that the Japanese process may have been similar to the Bessemer process, but cautions that alternative explanations are also plausible. William Kelly may have independently discovered the process before Bessemer 's patent. In the early 1850s, the American inventor William Kelly experimented with a method similar to the Bessemer process. Wagner writes that Kelly may have been inspired by techniques introduced by Chinese ironworkers hired by Kelly in 1854. When Bessemer 's patent for the process was reported by Scientific American, Kelly responded by writing a letter to the magazine. In the letter, Kelly states that he had previously experimented with the process and claimed that Bessemer knew of Kelly 's discovery. He wrote that `` I have reason to believe my discovery was known in England three or four years ago, as a number of English puddlers visited this place to see my new process. Several of them have since returned to England and may have spoken of my invention there. '' Sir Henry Bessemer described the origin of his invention in his autobiography written in 1890. During the outbreak of the Crimean War, many English industrialists and inventors became interested in military technology. According to Bessemer, his invention was inspired by a conversation with Napoleon III in 1854 pertaining to the steel required for better artillery. Bessemer claimed that it `` was the spark which kindled one of the greatest revolutions that the present century had to record, for during my solitary ride in a cab that night from Vincennes to Paris, I made up my mind to try what I could to improve the quality of iron in the manufacture of guns. '' At the time steel was used to make only small items like cutlery and tools, but was too expensive for cannons. Starting in January 1855 he began working on a way to produce steel in the massive quantities required for artillery and by October he filed his first patent related to the Bessemer process. He patented the method a year later in 1856. According to his autobiography Bessemer was working with an ordinary reverberatory furnace but during a test, some pieces of pig iron were jostled off the side of the ladle, and were left above the ladle in the furnace 's heat. When Bessemer went to push them into the ladle, he found that they were steel shells : the hot air alone had converted the outsides of the iron pieces to steel. This crucial discovery led him to completely redesign his furnace so that it would force high - pressure air through the molten iron using special air pumps. Intuitively this would seem to be folly because it would cool the iron. Instead, the oxygen in the forced air ignited silicon and carbon impurities in the iron, starting a positive feedback loop. As the iron became hotter, more impurities burned off, making the iron even hotter and burning off more impurities, producing a batch of hotter, purer, molten iron, which converts to steel more easily. Henry Bessemer Bessemer licensed the patent for his process to four ironmasters, for a total of £ 27,000, but the licensees failed to produce the quality of steel he had promised -- it was `` rotten hot and rotten cold '', according to his friend, William Clay -- and he later bought them back for £ 32,500. His plan had been to offer the licenses to one company in each of several geographic areas, at a royalty price per ton that included a lower rate on a proportion of their output in order to encourage production, but not so large a proportion that they might decide to reduce their selling prices. By this method he hoped to cause the new process to gain in standing and market share. He realised that the technical problem was due to impurities in the iron and concluded that the solution lay in knowing when to turn off the flow of air in his process so that the impurities were burned off but just the right amount of carbon remained. However, despite spending tens of thousands of pounds on experiments, he could not find the answer. Certain grades of steel are sensitive to the 78 % nitrogen which was part of the air blast passing through the steel. Bessemer was sued by the patent purchasers who could n't get it to work. In the end Bessemer set up his own steel company because he knew how to do it, even though he could not convey it to his patent users. Bessemer 's company became one of the largest in the world and changed the face of steel making. The solution was first discovered by English metallurgist Robert Forester Mushet, who had carried out thousands of experiments in the Forest of Dean. His method was to first burn off, as far as possible, all the impurities and carbon, then reintroduce carbon and manganese by adding an exact amount of spiegeleisen. This had the effect of improving the quality of the finished product, increasing its malleability -- its ability to withstand rolling and forging at high temperatures and making it more suitable for a vast array of uses. The first company to license the process was the Manchester firm of W & J Galloway, and they did so before Bessemer announced it at Cheltenham in 1856. They are not included in his list of the four to whom he refunded the license fees. However, they subsequently rescinded their license in 1858 in return for the opportunity to invest in a partnership with Bessemer and others. This partnership began to manufacture steel in Sheffield from 1858, initially using imported charcoal pig iron from Sweden. This was the first commercial production. Sidney Gilchrist Thomas, a Londoner with a Welsh father, was an industrial chemist who decided to tackle the problem of phosphorus in iron, which resulted in the production of low grade steel. Believing that he had discovered a solution, he contacted his cousin, Percy Gilchrist, who was a chemist at the Blaenavon ironworks. The manager at the time, Edward Martin, offered Sidney equipment for large - scale testing and helped him draw up a patent that was taken out in May, 1878. Sidney Gilchrist Thomas 's invention consisted of using dolomite or sometimes limestone linings for the Bessemer converter rather than clay, and it became known as the ' basic ' Bessemer rather than the ' acid ' Bessemer process. An additional advantage was that the processes formed more slag in the converter, and this could be recovered and used very profitably as a phosphate fertilizer. Patent battles Patents of such value did not escape criticism, and invalidity was urged against them on various grounds. But Bessemer was able to maintain them intact without litigation, though he found it advisable to buy up the rights of one patentee, Robert Forester Mushet. In the case of Mushet, he was assisted by the patent being allowed to lapse in 1859 through non-payment of fees. Mushet 's procedure was not essential and Bessemer proved this in 1865 by exhibiting a series of steel samples made using his process alone, but the value of the procedure was shown by its near universal adoption in conjunction with the Bessemer process. Whether or not Mushet 's patents could have been sustained is not known, but in 1866 Robert Mushet 's 16 - year - old daughter travelled to London to confront Henry Bessemer at his offices, arguing that Bessemer 's success was based on the results of her father 's work. Bessemer decided to pay Mushet an annual pension of £ 300 ( equivalent to £ 26,000 in 2016 ), a very considerable sum, which he paid for 25 years. In 1866, Bessemer also provided finance for Zerah Colburn, the American locomotive engineer and journalist, to start a new weekly engineering newspaper called Engineering based in Bedford Street, London. It was not until many years later that the name of Colburn 's benefactor was revealed. Before Engineering was launched, Colburn, through the pages of The Engineer, had given support to Bessemer 's work on steel and steelmaking. Importance Bessemer furnace in operation in Youngstown, Ohio, 1941. The Bessemer process revolutionized steel manufacture by decreasing its cost, from £ 40 per long ton to £ 6 -- 7 per long ton, along with greatly increasing the scale and speed of production of this vital raw material. The process also decreased the labor requirements for steel - making. Before it was introduced, steel was far too expensive to make bridges or the framework for buildings and thus wrought iron had been used throughout the Industrial Revolution. After the introduction of the Bessemer process, steel and wrought iron became similarly priced, and some users, primarily railroads, turned to steel. Quality problems, such as brittleness caused by nitrogen in the blowing air, prevented Bessemer steel from being used for many structural applications. Open - hearth steel was suitable for structural applications. Steel greatly improved the productivity of railroads. Steel rails lasted ten times longer than iron rails. Steel rails, which became heavier as prices fell, could carry heavier locomotives, which could pull longer trains. Steel rail cars were longer and were able to increase the freight to car weight from 1 : 1 to 2 : 1. As early as 1895 in the UK it was being noted that the heyday of the Bessemer process was over and that the open hearth method predominated. The Iron and Coal Trades Review said that it was `` in a semi-moribund condition. Year after year, it has not only ceased to make progress, but it has absolutely declined. '' It has been suggested, both at that time and more recently, that the cause of this was the lack of trained personnel and investment in technology rather than anything intrinsic to the process itself. For example, one of the major causes of the decline of the giant ironmaking company Bolckow Vaughan of Middlesbrough was its failure to upgrade its technology. The basic process, the Thomas - Gilchrist process, remained longer in use, especially in Continental Europe, where iron ores were of high phosphorus content and open hearth process was not able to remove all phosphorus ; almost all inexpensive construction steel in Germany was produced with this method in the 1950s and 1960s. It was eventually superseded by basic oxygen steelmaking. The Bessemer process in the United states While visiting Europe to obtain information on shipbuilding, armour, and armaments from 1862 to 1863, Alexander Lyman Holley visited Bessemer 's Sheffield works, and expressed interest in licensing the process for use in the US. Upon returning to the US, Holley met with noted inventor John Ericsson, who referred Holley to a pair of businessmen who had helped him build the Civil War ironclad USS Monitor, John F. Winslow and John Augustus Griswold. With Winslow and Griswold 's support, Holley returned to England in 1863, and paid Bessemer £ 10,000 to license the technology. The trio began setting up a mill in Troy, New York in 1865. The factory contained a number of Holley 's innovations that greatly improved productivity over Bessemer 's factory in Sheffield, and the owners gave a successful public exhibition in 1867. The Troy factory attracted the attention of the Pennsylvania Railroad, which wanted to use the new process to manufacture steel rail. It funded Holley 's second mill as part of its Pennsylvania Steel subsidiary. Between 1866 and 1877, the partners were able to license a total of 11 Bessemer steel mills. One of the investors they attracted was Andrew Carnegie, who saw great promise in the new steel technology after a visit to Bessemer in 1872, and saw it as a useful adjunct to his existing businesses, the Keystone Bridge Company and the Union Iron Works. Holley built the new steel mill for Carnegie, and continued to improve and refine the process. The new mill, known as the Edgar Thomson Steel Works, opened in 1875, and started the growth of the United States as a major world steel producer. William Walker Scranton, manager and owner of the Lackawanna Iron & Coal Company in Scranton, Pennsylvania, had also investigated the process in Europe. He built a mill in 1876 using the Bessemer process for steel rails and quadrupled his production. Obsolescence In the U.S., commercial steel production using this method stopped in 1968. It was replaced by processes such as the basic oxygen ( Linz - Donawitz ) process, which offered better control of final chemistry. The Bessemer process was so fast ( 10 -- 20 minutes for a heat ) that it allowed little time for chemical analysis or adjustment of the alloying elements in the steel. Bessemer converters did not remove phosphorus efficiently from the molten steel ; as low - phosphorus ores became more expensive, conversion costs increased. The process permitted only limited amount of scrap steel to be charged, further increasing costs, especially when scrap was inexpensive. Use of electric arc furnace technology competed favourably with the Bessemer process resulting in its obsolescence. Basic oxygen steelmaking is essentially an improved version of the Bessemer process ( decarburization by blowing oxygen as gas into the heat rather than burning the excess carbon away by adding oxygen carrying substances into the heat ). The advantages of pure oxygen blast over air blast was known to Henry Bessemer, but the 19th - century technology was not advanced enough to allow for the production of the large quantities of pure oxygen to make it economically feasible for use. See also Engineering portal Cementation ( metallurgy ) process Methods of crucible steel production Open hearth furnace, the Siemens - Martin process Open - hearth furnace process References Jump up ^ Ponting, Clive ( 2000 ), World History, A New Perspective, Pimlico, ISBN 0 - 7126 - 6572 - 2 ^ Jump up to : Needham, Joseph ( 2008 ). Science and civilisation in China, Volume 5, Part 7 ( 1. publ. ed. ). Cambridge, UK : Cambridge University Press. pp. 261 -- 5. ISBN 9780521875660. ^ Jump up to : Tanner, Harold ( 2009 ). China : A History. Hackett Publishing. p. 218. ISBN 0 - 87220 - 915 - 6. ^ Jump up to : Wagner, Donald ( 2008 ). Science and Civilisation in China : Vol. 5, Part 11 : Ferrous Metallurgy. Cambridge University Press. pp. 363 -- 5. ISBN 978 - 0 - 521 - 87566 - 0. ^ Jump up to : Wagner, Donald ( 2008 ). Science and Civilisation in China : Vol. 5, Part 11 : Ferrous Metallurgy. Cambridge University Press. p. 361. ISBN 978 - 0 - 521 - 87566 - 0. Jump up ^ `` Bessemer process ''. Britannica. 2. Encyclopædia Britannica. 2005. p. 168. Jump up ^ Gordon, Robert B. ( 2001 ). American Iron, 1607 -- 1900. JHU Press. pp. 221 --. ISBN 978 - 0 - 8018 - 6816 - 0. Jump up ^ http://www.gutenberg.org/files/29633/29633-h/29633-h.htm Jump up ^ http://www.uh.edu/engines/epi762.htm Jump up ^ Shaping Technology / building Society : Studies in Sociotechnical Change. MIT Press. pp. 112 --. ISBN 978 - 0 - 262 - 26043 - 5. Jump up ^ ( 1 ) Jump up ^ `` Purchasing Power of British Pounds from 1264 to Present ''. 2009. Retrieved January 14, 2011. ^ Jump up to : Hartwell, Robert ( March 1966 ). `` Markets, Technology, and the Structure of Enterprise in the Development of the Eleventh - Century Chinese Iron and Steel Industry ''. The Journal of Economic History. 26 ( 1 ) : 54. ISSN 0022 - 0507. JSTOR 2116001. Jump up ^ Wertime, Theodore A. ( 1962 ). The coming of the age of steel. University of Chicago Press. Jump up ^ Temple, Robert K.G. ( 1999 ). The Genius of China : 3000 years of science, discovery and invention. London : Prion. p. 49. ISBN 9781853752926. ^ Jump up to : Erickson, Charlotte ( 1986 ) ( 1959 ). British industrialists : steel and hosiery 1850 -- 1950. Cambridge University Press. pp. 141 -- 142. ISBN 0 - 566 - 05141 - 9. Jump up ^ Bessemer, Sir Henry ( 1905 ). Sir Henry Bessemer, F.R.S. Offices of `` Engineering '',. p172. Jump up ^ Anstis 1997, p. 147. Jump up ^ J.E. Gordon, `` The new science of strong materials '', Penguin books. Jump up ^ `` Mushet, Robert Forester ''. Dictionary of National Biography. London : Smith, Elder & Co. 1885 -- 1900. Jump up ^ Anstis 1997, p. 140. Jump up ^ Bessemer, Sir Henry ( 1905 ). An Autobiography. London : Engineering. pp. 176, 180. Jump up ^ Blaenavon World Heritage Site : Blaenavon and the ' Gilchrist - Thomas ' Process Archived December 12, 2013, at the Wayback Machine. Jump up ^ Company, Lewis Publishing ( 1908 - 01 - 01 ). A century and a half of Pittsburg and her people. Lewis Pub. Co. p. 41. Jump up ^ Chapter 18 Manganese in Steel Making Jump up ^ Rosenberg, Nathan ( 1982 ). Inside the Black Box : Technology and Economics. Cambridge, New York : Cambridge University Press. p. 90. ISBN 0 - 521 - 27367 - 6. Jump up ^ Misa, Thomas J. ( 1999 ) ( 1995 ). A Nation of Steel : The Making of Modern America, 1865 -- 1925. Johns Hopkins studies in the history of technology. Baltimore, Md. : The Johns Hopkins University Press. ISBN 0 - 8018 - 6052 - 0. OCLC 540692649. Chapter 1 online. Jump up ^ Rosenberg, Nathan ( 1982 ). Inside the Black Box : Technology and Economics. Cambridge, New York : Cambridge University Press. pp. 60, 69. ISBN 0 - 521 - 27367 - 6. Jump up ^ Payne, P.L. ( 1968 ). `` Iron and steel manufactures ''. In Aldcroft, Derek H. The development of British industry and foreign competition, 1875 -- 1914 ; studies in industrial enterprise. London : George Allen & Unwin. pp. 92 -- 94, 97. OCLC 224674. Jump up ^ Abe, E. The Technological Strategy of a Leading Iron and Steel Firm : Bolckow Vaughan Co. Ltd : Late Victorian Industrialists Did Fail. Business History, 1996, Vol. 38, No. 1, pages 45 -- 76. Jump up ^ Rail that Survived Demolition by `` Lawrence of Arabia '' : An Analysis Jump up ^ ( 2 ) Jump up ^ Thomas J. Misa, A Nation of Steel : The Making of Modern America, 1865 -- 1925 ( 1995 ) : chapter on Holley and Bessemer process online Jump up ^ Cheryl A. Kashuba, `` William Walker led industry in the city '', The Times - Tribune, 11 July 2010, accessed 23 May 2016 Bibliography Anstis, Ralph ( 1997 ), Man of Iron, Man of Steel : Lives of David and Robert Mushet, Albion House, ISBN 0 - 9511371 - 4 - X External links Wikimedia Commons has media related to Bessemer converter. `` Progress in the Manufacture of Steel '' in Popular Science Monthly Volume 19, October 1881 `` Bessemer 's explanation of his process ''. The Engineer. 15 August 1856. `` How the Modern Steel Furnace Does Its Work ''. Popular Science : 30 -- 31. February 1919. Iron and steel production History of ferrous metallurgy List of steel producers Iron production ( Ironworks ) Smelting Bloomery ( produces sponge iron ) Blast furnace ( produces pig iron ) Cold blast Hot blast Anthracite iron Direct reduced iron Secondary Wrought iron ( via Finery forge or Reverberatory Puddling Furnace ) Cast iron ( via Cupola furnace or Induction furnace ) Steelmaking ( Steel mill ) Primary ( Pre-1850 ) Pattern welding ( Damascus steel ) Crucible steel Tatara furnace Cementation process Primary ( Post-1850 ) Bessemer process Open hearth furnace Electric arc furnace Basic oxygen process Secondary Electro - slag remelting Vacuum arc remelting Argon oxygen decarburization Production by country Bangladesh China Italy Luxembourg Retrieved from `` https://en.wikipedia.org/w/index.php?title=Bessemer_process&oldid=813121467 '' Categories : English inventions Steelmaking Metallurgical processes Hidden categories : Articles incorporating Cite DNB template Webarchive template wayback links Wikipedia articles needing clarification from April 2011 All articles with unsourced statements Articles with unsourced statements from April 2011 Articles with unsourced statements from January 2016 Talk Contents About Wikipedia Български Català Čeština Dansk Deutsch Español Euskara Français Gaeilge Galego 한국어 हिन्दी Hrvatski Italiano ಕನ್ನಡ ქართული Lëtzebuergesch Magyar Nederlands 日本 語 Norsk Oʻzbekcha / ўзбекча Polski Português Русский Slovenčina Srpskohrvatski / српскохрватски Suomi Svenska தமிழ் తెలుగు Türkçe Українська 中文 Edit links This page was last edited on 1 December 2017, at 22 : 21. Text is available under the Creative Commons Attribution - ShareAlike License ; additional terms may apply. By using this site, you agree to the Terms of Use and Privacy Policy. Wikipedia ® is a registered trademark of the Wikimedia Foundation, Inc., a non-profit organization. About Wikipedia

Question: who developed a method to mass-produce steel in america
Answer: Henry Bessemer